Crystalline perfection of an aluminium single crystal determined by neutron diffraction


 Edgar Horton
 2 years ago
 Views:
Transcription
1 Journal of Applied Crystallography ISSN Editor: Anke R. KaysserPyzalla Crystalline perfection of an aluminium single crystal determined by neutron diffraction Sabrina Metairon, Carlos Benedicto Ramos Parente, Vera Lucia Mazzocchi and Thierry Jacques Lemaire J. Appl. Cryst. (2011). 44, Copyright c International Union of Crystallography Author(s) of this paper may load this reprint on their own web site or institutional repository provided that this cover page is retained. Republication of this article or its storage in electronic databases other than as specified above is not permitted without prior permission in writing from the IUCr. For further information see Journal of Applied Crystallography covers a wide range of crystallographic topics from the viewpoints of both techniques and theory. The journal presents papers on the application of crystallographic techniques and on the related apparatus and computer software. For many years, the Journal of Applied Crystallography has been the main vehicle for the publication of smallangle scattering papers and powder diffraction techniques. The journal is the primary place where crystallographic computer program information is published. Crystallography Journals Online is available from journals.iucr.org J. Appl. Cryst. (2011). 44, Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal
2 Journal of Applied Crystallography ISSN Received 17 December 2010 Accepted 16 June 2011 Crystalline perfection of an aluminium single crystal determined by neutron diffraction Sabrina Metairon, a Carlos Benedicto Ramos Parente, a * Vera Lucia Mazzocchi a and Thierry Jacques Lemaire b a Instituto de Pesquisas Energéticas e Nucleares (IPENCNEN/SP), São Paulo, SP, Brazil, and b Universidade Federal da Bahia (UFBA), Salvador, BA, Brazil. Correspondence # 2011 International Union of Crystallography Printed in Singapore all rights reserved In this work, a study of the crystalline perfection of an aluminium single crystal is presented. The study shows that, from threedimensional neutron diffraction rocking curves, it is possible to characterize the individual crystalline domains of a multidomain crystal. From a macroscopic point of view, the determination of the domains allows an evaluation of the crystalline perfection of the crystal under study. Threedimensional rocking curves have been obtained by neutron diffraction from a large mosaic aluminium crystal. Construction of a contour map of individual domains made it easier to determine the breadth and relative intensity of each domain. The angular distances between domains were also determined. 1. Introduction Baldochi et al. (1994) carried out a study of the crystalline quality of large Czochralskigrown barium lithium fluoride (BaLiF 3 ) single crystals. In that study, certain characteristics of neutron diffraction intensity curves (rocking curves) were correlated with several parameters involved in the growth method. As pointed out by the authors, neutrons are better than Xrays for this purpose since they give information about the bulk of the crystal. A neutron beam has, in general, a large crosssectional area and a sample can be completely immersed in it. Furthermore, neutrons are highly penetrating particles for most materials. These two characteristics together make it easier to observe all crystalline domains of a single crystal, particularly if it is bulky. An Xray beam, on the other hand, is much less penetrating than a neutron beam and has, in general, a small crosssectional area. Thus, Xray diffraction gives information about a very small surface portion of a large crystal. A single domain is then observed, unless the beam impinges upon a domain boundary. It is possible to use an Xray beam to observe many crystalline domains of a multidomain crystal, but a careful and exhaustive procedure must be adopted in order to sweep the entire surface of the crystal, which is undoubtedly very time consuming. Even then, domains located in the innermost part of the crystal will never be observed unless etching is used in the analysis. Although the methodology employed in the study of Baldochi et al. (1994) led to useful results, it is not suitable for a complete characterization of the crystalline domains of a sample. This is due to the fact that the methodology used twodimensional instead of threedimensional neutron diffraction rocking curves. In general, a twodimensional rocking curve shows only a few crystalline domains; such domains appear as overlapping peaks. Except for those cases where the domains are closely aligned in the direction of the measurement, only a threedimensional I! rocking curve can show all the domains of a crystal (I is the observed intensity of an hkl reflection, and! and are two orthogonal rotations around axes that are both orthogonal to the scattering vector of the reflection). The domains are located at different regions in the! grid. In principle, with a threedimensional rocking curve it is possible to determine the number of domains, their relative intensities, the breadth of each one and the angular dispersion between them. From a macroscopic point of view, the determination of such characteristics allows an evaluation of the crystalline perfection of the crystal under study. The present work establishes a methodology for the analysis of the crystalline quality of single crystals using threedimensional neutron diffraction rocking curves. J. Appl. Cryst. (2011). 44, doi: /s Experimental A twodimensional rocking curve can be obtained by turning the crystal around the! axis of an Eulerian cradle while the intensity I of an hkl reflection is measured. During the measurement, the neutron detector remains in a fixed position at the scattering angle 2 hkl relative to the incident beam. This is the socalled movingcrystal stationarydetector procedure. It corresponds to an! scan in the normalbeam equatorial geometry (Arndt & Willis, 1966). A threedimensional I! rocking curve is formed using a set of twodimensional I! rocking curves measured at different values of, obtained by stepping this angle in convenient intervals. Fig. 1 is a schematic representation of the rotations used to obtain a threedimensional I! rocking curve. To carry out the measurements, an experimental arrangement was assembled on the multipurpose neutron diffractelectronic reprint
3 ometer installed at the IEAR1 research reactor at IPEN. At the time of the measurements, the reactor was operating at a power of 2 MW thermal. The 200 reflection of a large mosaic copper single crystal was used to obtain a monochromatic beam. At a takeoff angle of , the wavelength was Å. The diffractometer was designed based on the normalbeam equatorial geometry. In the arrangement used for the rockingcurve measurements, the monochromatic beam Soller collimator was replaced with a special collimator which limits the vertical and horizontal divergences equally. This is the same collimator used to perform neutron multiple diffraction measurements on the instrument (Mazzocchi & Parente, 1994, 1998). The beam cross section for this collimator is cm and the vertical and horizontal divergences are ca The experimental arrangement also included a fivecircle goniometer, which resembles an Eulerian cradle except that it has an extra horizontal axis () appropriate for use in neutron multiple diffraction measurements (Mazzocchi & Parente, 1994). The crystal used in the measurements was a mosaic aluminium crystal shaped as a square plate, cm, and oriented with the (111) planes parallel to the square face. It was attached firmly to a goniometer head with the [111] direction approximately parallel to its central axis. The goniometer head was fastened to the axis of the fivecircle goniometer. This axis was rotated around the axis until it and the axis became coaxial. Careful orientation of the crystal in the neutron beam, in order to obtain the maximum intensity of the 111 reflection, preceded the measurements. The twodimensional rocking curves were obtained by scanning! in steps of 0.05 with a count time of 2 min for each step. Although the area of the crystal surface was larger than the neutron beam cross section, the measurements were carried out without any sweep of the crystal in the beam. To obtain the threedimensional rocking curve, the angle was varied in steps of 0.5. Such a large step was possible since the scale is stretched owing to the geometry of the measurements (see x3.4). Scans in both angular directions! and were made large enough to extend the background for a few degrees on both sides of the curves. To determine the instrumental broadenings for both! and directions, we used a lithium fluoride (LiF) single crystal grown by the Czochralski method (Hagenmuller, 1972). Two twodimensional 200 rocking curves were measured, one for each direction,! or. The rocking curve in the direction was measured after a 90 rotation of the crystal around the Figure 1 A schematic representation of the rotations! and used to obtain a threedimensional I! rocking curve. axis. This rotation was done in order to ensure that approximately the same region of the crystal used to obtain the instrumental broadening in the! direction was also used to obtain the instrumental broadening in the direction. A careful Gaussian fit to both rocking curves showed that the crystal had several domains. The domain with the smallest values of the full widths at halfmaximum (FWHMs) gave the values for the instrumental broadening. These are both represented by K and were and 0.913, respectively, for the! and directions. 3. Data treatment The purpose of the data treatment was to obtain the intrinsic threedimensional crystalline domains of the aluminium crystal. For this purpose, each experimental twodimensional rocking curve was fitted with Gaussians, followed by deconvolution of the Gaussians. Both processes were first applied to the rocking curves obtained in the! direction and then to those obtained in the direction, the latter curves being extracted from the set of the former curves. An interpolation of points (Press et al., 1994) was performed prior to the deconvolution in order to guarantee better quality of the results. Contour maps were constructed with the deconvoluted data, allowing an easier characterization of the crystalline domains. All procedures employed in the data treatment are briefly described below Deconvolution of Gaussians Deconvolution (or unfolding) of instrumental broadening from an experimental curve is, in general, a hard task with no guarantee of success. According to Press et al. (1994), apart from some mathematical problems, the process of deconvolution has other practical shortcomings. It is quite sensitive to noise in the input data and to the accuracy to which the response function is known. In this work, all such problems were overcome by simply assuming that the data must be fitted with Gaussian functions prior to the application of the deconvolution process. The process is then individually applied to each Gaussian fit. In this case, deconvolution becomes a straightforward mathematical process, without any additional difficulties. Clearly, this kind of solution is possible only because experimental neutron diffraction rocking curves can be fitted with Gaussian functions with excellent results. A computer program was written in order to deconvolute the rocking curves. In a single run of the program, all Gaussians of a twodimensional rocking curve can be deconvoluted. During the run, the deconvolution process is applied individually to each Gaussian according to the sequence in which they are listed in the input data. The output from the program gives the data for the deconvoluted rocking curve, as well as the parameters of each deconvoluted Gaussian. The program was first applied to all twodimensional I! rocking curves, using the instrumental broadening in the! direction. Twodimensional I rocking curves were then extracted from the set formed by the deconvoluted I! rocking curves, one for 682 Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal J. Appl. Cryst. (2011). 44,
4 each value of! in its interval of variation. In a similar manner, using the instrumental broadening in the direction, I rocking curves were deconvoluted. It should be noted that each interpolated point generates a new rocking curve in the transverse direction. This is valid for both! and directions and causes a substantial increase in the number of rocking curves to be fitted and deconvoluted. The threedimensional rocking curve constructed from the raw experimental data obtained with the aluminium crystal is shown in Fig. 2(a). The threedimensional rocking curve shown in Fig. 2(b) was constructed after interpolation and deconvolution of the twodimensional rocking curves of Fig. 2(a), forming the deconvoluted threedimensional I! rocking curve for the aluminium crystal. Interpolation of points is clearly seen when comparing the figures. An appreciable change in the twodimensional rocking curves that form the surface enveloping the threedimensional curve is also clearly seen Fitting of data The fits were performed by means of a computer program that adjusts Gaussians to an experimental curve, using the leastsquares method in the fitting process. It is not worthwhile to give a more detailed description of this program here. It belongs to a well known class of computer programs which perform the fitting of experimental curves with suitable mathematical functions. The program gives as output all three parameters of each Gaussian found in the fit, namely position, maximum intensity and FWHM. It also gives the area under each Gaussian, as well as the intensity points forming it. Parameters and areas are given with their standard deviations. An overall standard deviation for the fit itself is also given. A serious drawback of this sort of program is that, in certain cases, the number of Gaussians to be specified for the fit becomes undefined. This happens when the curve to be fitted has several overlapping peaks with poor separation between them. This is the case in this work. A better description of the problem and its solution is given below. During fitting of the numerous rocking curves we have verified that, after a certain number of Gaussians, the agreement between experimental and fitted curves experiences no substantial improvement. When the number of Gaussians becomes too large, the fit becomes erratic, although without spoiling the agreement. Figs. 3(a), 3(b) and 3(c) are plots of the overall standard deviation versus number of Gaussians n, obtained by fitting neighbouring rocking curves with, successively, n = 1, 2, 3, 4 or 5 Gaussians. They show how the agreement behaves with increasing n. Plots in the figures were obtained with I! rocking curves measured at, respectively, = 89.5, 90 and It is remarkable how changes by two orders of magnitude when n goes from 1 to 3 for all three rocking curves. From n = 3 onwards tends to stabilize. For this particular case, the number of Gaussians to be adopted should be at least n = 3. However, a better choice of n still depends on a qualitative evaluation of the fits, which should take into account how a Gaussian is altered when passing from one rocking curve to a neighbouring one. As a general rule for a nondeformed domain, the parameters of successive Gaussians, in particular the maximum intensity and FWHM, should change monotonically on both sides of the maximum. To ensure that the results of the fitting process are reliable, the fits must be checked continuously in order to verify if the domains follow the above behaviour. It is important to mention that, depending on the particular case, the procedure for the determination of n must be applied again when domains Figure 2 Threedimensional I! rocking curves constructed using (a) the raw experimental data obtained from the aluminium crystal and (b) after interpolation and deconvolution. J. Appl. Cryst. (2011). 44, Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal 683
5 appear or disappear in the sequence of rocking curves. As an illustration of the procedures described above, three Gaussians were chosen to initiate the fitting in the cases corresponding to Fig Contour maps A threedimensional plot, like that of Fig. 2(b), does not allow a complete visualization of the rocking curve. Some details are always missing, unless the plot is rotated around a vertical axis and several plots are shown. For a better visualization of a threedimensional rocking curve, a contour map must be constructed with the same data as used in the threedimensional plot Reduction of the v scale During determination of the instrumental broadening, we observed that the breadths of the rocking curves, measured in the directions! and, were very different. The breadth in the direction was ca 16 times that in the! direction. Such a large difference could not be attributed to intrinsic characteristics of the crystal. In fact, as mentioned above, the crystal was rotated by 90 for the measurement in the direction to ensure that essentially the same crystalline region was observed in both measurements. If not exactly the same, these regions were very alike in their characteristics. However, the enlargement of the rocking curve in the direction is in fact due to an enhancement of the Lorentz factor (Metairon, 1999). This factor depends on the inclination, with respect to the surface of the Ewald sphere, of the trajectory described by a reciprocal lattice point during rocking of the crystal. The more inclined the trajectory, the more the rocking curve is enlarged. In an! rocking of the crystal, the trajectory is almost perpendicular to the sphere and a small enlargement occurs. On the other hand, in a rocking the reciprocal lattice point approximates to the surface of the sphere at a grazing incidence and an enlarged rocking curve results (Rossmanith, 1986; Metairon, 1999). In order to reduce the enlargement in the direction a correction factor f corr was determined, which causes reduction of the scale. The reduction is such that the breadths of the twodimensional domains in one direction become of the same order of magnitude as those in the other direction. The correction factor was calculated by dividing the FWHM of a rocking curve measured in the! direction by the FWHM of one measured in the direction, provided these rocking curves were measured in the same crystalline direction according to the procedure adopted in the determination of the instrumental broadening. The value of the correction factor for the aluminium crystal is f corr = Reduction of the scale is achieved by calculating the correct using the expression corr =( max )f corr, where max is the coordinate of the point of maximum intensity in the threedimensional rocking curve. Fig. 4 shows the contour map constructed for the aluminium crystal. In contrast with Figs. 2(a)and2(b), Fig. 4 is plotted on a reduced scale where max =90.The! scale in the contour map is equal to that used in Fig Individual characterization of domains The contour map of Fig. 4 contains all the information required to allow an evaluation of the crystalline quality of the aluminium crystal. Nevertheless, it is not a useful source of information when individual characterization of the crystalline Figure 3 The overall standard deviation () versus number of Gaussians (n) obtained by fitting I! rocking curves, measured at (a) = 89.5,(b) = 90 and (c) = 90.5, with one to five Gaussians. Figure 4 A contour map constructed for the aluminium crystal after deconvolution in both! and directions. The scale was reduced using max =90 and a correction factor f corr = Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal J. Appl. Cryst. (2011). 44,
6 domains and the relationships between them are sought. To achieve this objective, a contour map of the individual domains must be constructed. The construction is carried out using data collected from the outputs of the computer program used for the deconvolutions. It should be noted that a deconvoluted threedimensional domain is formed via a certain number of deconvoluted Gaussians. Using the three parameters defining each such Gaussian, it is possible to individualize the domain in the contour map. It is worth mentioning that the direction assumed for the construction,! or, is irrelevant provided the same direction is used for the entire contour map. Extending this procedure to all domains of the crystal, a contour map of individual domains can be constructed. Fig. 5 shows a contour map of the individual domains constructed for the aluminium crystal. It combines the five threedimensional domains found in the analysis of the crystal. Taking domain No. 3 (the highest one) as reference, the intensity levels assigned to the contour lines vary according to the following: the blank region on the map is zero, the first contour line corresponds to counts, the second to , the third to , the fourth to and so on. The eleventh and last contour line corresponds to counts. To ascertain the intensity level of any other domain is a matter of finding the number of the contour line forming it. Using the contour map of Fig. 5, the angular distances between the individual domains and their relative intensities and breadths can be determined. The procedures used to acquire this information and the results obtained are presented below. 4. Results 4.1. Breadths of the domains The FWHM was assumed to be an adequate representation of the breadth of a domain. Since the domains are threedimensional, two values for the FWHM were considered, corresponding to directions! and. They are readily determined by first tracing orthogonal straight lines, intersecting at the point of maximum intensity of a domain. The lines are traced parallel to the! and axes. The FWHMs in both directions are determined when the straight lines encounter the contour line corresponding to half of the maximum intensity. Fig. 6 shows domain No. 3 of Fig. 5. In contrast with Fig. 5, the scale used to define the 11 contour lines in Fig. 6 is formed by the intensity levels 2982, 5965, 8947, , , , , , , and counts. Using the values corresponding to the maximum intensity (35 787) and half of the maximum intensity (17 893), the FWHMs for directions! and were determined following the procedure described above. They are indicated in Fig. 6 by! and and their values listed in Table 1, together with the values determined for the other domains. The corresponding values for the mosaic spreads! and are also listed in Table Angular distances between the domains In a contour map like that of Fig. 5, the angular distance separating two domains is represented by a line segment uniting the points of maximum intensity in the domains. Owing to the fact that! and are angular scales, any line segment traced in the map is actually an arc of circle. Metairon (1999) observed that, for the determination of the angular distances, a spherical right triangle should be considered. In such a triangle, if is the hypotenuse, i.e. the angular distance to be determined,! and are the catheti, i.e. its components along directions! and, andw (= 90 ) is the opposite angle to arc, then according to the cosine law (Spiegel, 1968) the following relationships can be written: Figure 5 A contour map for the aluminium crystal, constructed with individual domains. Figure 6 Determination of the FWHM of domain No. 3 of Fig. 5, for both! and directions (! and, respectively). J. Appl. Cryst. (2011). 44, Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal 685
7 Table 1 FWHM () and standard deviation () for both! and directions, determined for the five crystalline domains of the aluminium crystal. Domain! ( ) ( )! ( ) ( ) Table 2 Angular distances () between the five domains found in the aluminium crystal. Domains! ( ) ( ) ( ) 1 and and and and and and and and and and cos ¼ cos! cos þ sin! sin cos W ¼ cos! cos : To calculate between two domains, the points of maximum intensity in the domains must first be localized in the! grid and then projected upon the axes! and. The angular lengths of the two line segments determined by the projections are then the values to be assigned to the rectangular components! and. With these two values, can be easily calculated using the expression above. Table 2 lists the distances calculated for the ten possible combinations between the domains of the aluminium crystal. The corresponding values for! and are also listed in Table 2. As pointed out by Metairon (1999), can also be calculated to a good approximation by assuming a planar right triangle and using the Pythagorean theorem, i.e. 2 =! 2 + 2, provided! and are sufficiently small (no more than a few degrees) Relative intensities The relative intensities of the domains were calculated using the areas of the deconvoluted twodimensional Gaussians that pass through the points of maximum intensity. Since the threedimensional domains exhibited a certain asymmetry, the two Gaussians oriented in directions! and were considered for each domain. The areas were calculated according to the well known formula A = I max, where the maximum intensity (I max ) and the FWHM () are given in the output of the program used for the deconvolutions. Finally, the arithmetic mean A m of the two areas was calculated and used in the determination of the relative intensity I r of the domains. Table 3 lists for each domain the areas A! and A, obtained for directions! and, respectively, the mean area A m, and the Table 3 Relative intensities (I r ) of the domains in the aluminium crystal. Domain A! A A m I r (%) relative intensity I r. It should be noted that domain No. 3 was taken as reference for the calculations. 5. Concluding remarks In this work, a methodology for analysing the crystalline perfection of single crystals has been presented. The use of neutron diffraction enables the determination of the intrinsic crystalline domains of a crystal, therefore allowing an evaluation of its macroscopic crystalline perfection. Some of the procedures adopted during the data treatment and the determination of the characteristics of the domains are merely suggestions of practical ways to obtain the results and they should not be regarded as the only or best method to be used. Other solutions can be found, particularly for the determination of the FWHMs of domains and their relative intensities. Even the deconvolution of rocking curves is not absolutely necessary, unless the intrinsic characteristics of the domains are desired. Deconvolution is applied, or not, depending on the particular analysis and the results expected from the analysis. It should be noted that, in this study, the aluminium crystal was larger than the neutron beam crosssectional area and no scanning was performed during the measurements (see x2). Taking into account the distance between the collimator exit and the sample (35 cm), the vertical and horizontal divergences, the beam dimensions, and the Bragg angle for reflection 111 (ca 14 ), we have calculated that approximately 60% of the crystal volume was immersed in the neutron beam during the measurements, but this has not impeded a good evaluation of the crystalline perfection of the crystal. Concerning its quality, it could be said that the aluminium crystal is not really a single crystal, although it was acquired as being one. The existence of five domains separated by angular distances ranging from to (see Table 2) corroborates the above assertion. Use of such a crystal in a given application will depend on the particular needs of the application. It is important to note that the user of a crystal is the best judge if its quality is adequate, or not, for an intended use. The authors are indebted to Dr Sonia L. Baldochi and Dr Izilda M. Ranieri, from the Crystal Growth Laboratory at IPENCNEN/SP, for providing the LiF single crystal used in this study. We are also grateful for financial support given by the International Atomic Energy Agency (IAEA, project No. 6974/R1/RB) and the Conselho Nacional de Desenvolvimento Científico e Tecnológico (CNPq) (contract No / Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal J. Appl. Cryst. (2011). 44,
8 FA). One of the authors (SM) acknowledges the grant of a fellowship by CNPq (contract No /941). References Arndt, U. W. & Willis, B. T. M. (1966). Single Crystal Diffractometry. Cambridge University Press. Baldochi, S. L., Mazzocchi, V. L., Parente, C. B. R. & Morato, S. P. (1994). Mater. Res. Bull, 29, Hagenmuller, P. (1972). Editor. Preparative Methods in Solid State Chemistry. New York, London: Academic Press. Mazzocchi, V. L. & Parente, C. B. R. (1994). J. Appl. Cryst. 27, Mazzocchi, V. L. & Parente, C. B. R. (1998). J. Appl. Cryst. 31, Metairon, S. (1999). MSc dissertation, Universidade de São Paulo, São Paulo, SP, Brazil. Press, W. H., Teukolsky, S. A., Vetterling, W. T. & Flannery, B. P. (1994). Numerical Recipes in Fortran: The Art of Scientific Computing, 2nd ed. Cambridge University Press. Rossmanith, E. (1986). Acta Cryst. A42, Spiegel, M. R. (1968). Mathematical Handbook of Formulas and Tables. Schaum s Outline Series. New York: McGraw Hill Book Company. J. Appl. Cryst. (2011). 44, Sabrina Metairon et al. Crystalline perfection of an aluminium single crystal 687
Xray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More informationSection 1.1. Introduction to R n
The Calculus of Functions of Several Variables Section. Introduction to R n Calculus is the study of functional relationships and how related quantities change with each other. In your first exposure to
More informationLAUE DIFFRACTION INTRODUCTION CHARACTERISTICS X RAYS BREMSSTRAHLUNG
LAUE DIFFRACTION INTRODUCTION Xrays are electromagnetic radiations that originate outside the nucleus. There are two major processes for Xray production which are quite different and which lead to different
More informationStudents will understand 1. use numerical bases and the laws of exponents
Grade 8 Expressions and Equations Essential Questions: 1. How do you use patterns to understand mathematics and model situations? 2. What is algebra? 3. How are the horizontal and vertical axes related?
More informationXRAY DIFFRACTION PROCEDURES
XRAY DIFFRACTION PROCEDURES For Polycrystalline and Amorphous Materials HAROLD P. KLUG HEAD OF THE DEPARTMENT OF RESEARCH IN CHEMICAL PHYSICS LEROY E. ALEXANDER SENIOR FELLOW IN XRAY DIFFRACTION Mellon
More informationwith functions, expressions and equations which follow in units 3 and 4.
Grade 8 Overview View unit yearlong overview here The unit design was created in line with the areas of focus for grade 8 Mathematics as identified by the Common Core State Standards and the PARCC Model
More informationIntroduction to XRay Powder Diffraction Data Analysis
Introduction to XRay Powder Diffraction Data Analysis Center for Materials Science and Engineering at MIT http://prism.mit.edu/xray An Xray diffraction pattern is a plot of the intensity of Xrays scattered
More informationChapter 8. Low energy ion scattering study of Fe 4 N on Cu(100)
Low energy ion scattering study of 4 on Cu(1) Chapter 8. Low energy ion scattering study of 4 on Cu(1) 8.1. Introduction For a better understanding of the reconstructed 4 surfaces one would like to know
More information11.1. Objectives. Component Form of a Vector. Component Form of a Vector. Component Form of a Vector. Vectors and the Geometry of Space
11 Vectors and the Geometry of Space 11.1 Vectors in the Plane Copyright Cengage Learning. All rights reserved. Copyright Cengage Learning. All rights reserved. 2 Objectives! Write the component form of
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationReflection and Refraction
Equipment Reflection and Refraction Acrylic block set, planeconcaveconvex universal mirror, cork board, cork board stand, pins, flashlight, protractor, ruler, mirror worksheet, rectangular block worksheet,
More informationBiggar High School Mathematics Department. National 5 Learning Intentions & Success Criteria: Assessing My Progress
Biggar High School Mathematics Department National 5 Learning Intentions & Success Criteria: Assessing My Progress Expressions & Formulae Topic Learning Intention Success Criteria I understand this Approximation
More informationLaue lens for Nuclear Medicine
Laue lens for Nuclear Medicine PhD in Physics Gianfranco Paternò Ferrara, 611013 Supervisor: prof. Vincenzo Guidi Sensors and Semiconductors Lab, Department of Physics and Earth Science, University of
More informationMA 323 Geometric Modelling Course Notes: Day 02 Model Construction Problem
MA 323 Geometric Modelling Course Notes: Day 02 Model Construction Problem David L. Finn November 30th, 2004 In the next few days, we will introduce some of the basic problems in geometric modelling, and
More informationELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES
ELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES The purpose of this lab session is to experimentally investigate the relation between electric field lines of force and equipotential surfaces in two dimensions.
More informationPowder diffraction and synchrotron radiation
Powder diffraction and synchrotron radiation Gilberto Artioli Dip. Geoscienze UNIPD CIRCe Center for Cement Materials single xl diffraction powder diffraction Ideal powder Powder averaging Textured sample
More informationA reinterpretation of the phase transitions in Na 2 CO 3
Acta Crystallographica Section B Structural Science ISSN 01087681 Editor: Carolyn P. Brock A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva and Gervais Chapuis Copyright International
More informationGEOMETRY COMMON CORE STANDARDS
1st Nine Weeks Experiment with transformations in the plane GCO.1 Know precise definitions of angle, circle, perpendicular line, parallel line, and line segment, based on the undefined notions of point,
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationFall 12 PHY 122 Homework Solutions #8
Fall 12 PHY 122 Homework Solutions #8 Chapter 27 Problem 22 An electron moves with velocity v= (7.0i  6.0j)10 4 m/s in a magnetic field B= (0.80i + 0.60j)T. Determine the magnitude and direction of the
More informationNonlinear Iterative Partial Least Squares Method
Numerical Methods for Determining Principal Component Analysis Abstract Factors Béchu, S., RichardPlouet, M., Fernandez, V., Walton, J., and Fairley, N. (2016) Developments in numerical treatments for
More informationSession 6 Area. area midline similar figures
Key Terms in This Session Session 6 Area Previously Introduced scale factor New in This Session area midline similar figures Introduction Area is a measure of how much surface is covered by a particular
More informationXray Diffraction and EBSD
Xray Diffraction and EBSD Jonathan Cowen Swagelok Center for the Surface Analysis of Materials Case School of Engineering Case Western Reserve University October 27, 2014 Outline Xray Diffraction (XRD)
More informationObjectives After completing this section, you should be able to:
Chapter 5 Section 1 Lesson Angle Measure Objectives After completing this section, you should be able to: Use the most common conventions to position and measure angles on the plane. Demonstrate an understanding
More informationKEANSBURG SCHOOL DISTRICT KEANSBURG HIGH SCHOOL Mathematics Department. HSPA 10 Curriculum. September 2007
KEANSBURG HIGH SCHOOL Mathematics Department HSPA 10 Curriculum September 2007 Written by: Karen Egan Mathematics Supervisor: Ann Gagliardi 7 days Sample and Display Data (Chapter 1 pp. 447) Surveys and
More informationInternational Year of Light 2015 TechTalks BREGENZ: Mehmet Arik WellBeing in Office Applications Light Measurement & Quality Parameters
www.ledprofessional.com ISSN 1993890X Trends & Technologies for Future Lighting Solutions ReviewJan/Feb 2015 Issue LpR 47 International Year of Light 2015 TechTalks BREGENZ: Mehmet Arik WellBeing in
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationAlgebra Geometry Glossary. 90 angle
lgebra Geometry Glossary 1) acute angle an angle less than 90 acute angle 90 angle 2) acute triangle a triangle where all angles are less than 90 3) adjacent angles angles that share a common leg Example:
More informationGeorgia Standards of Excellence Curriculum Map. Mathematics. GSE 8 th Grade
Georgia Standards of Excellence Curriculum Map Mathematics GSE 8 th Grade These materials are for nonprofit educational purposes only. Any other use may constitute copyright infringement. GSE Eighth Grade
More informationEXPERIMENTAL ERROR AND DATA ANALYSIS
EXPERIMENTAL ERROR AND DATA ANALYSIS 1. INTRODUCTION: Laboratory experiments involve taking measurements of physical quantities. No measurement of any physical quantity is ever perfectly accurate, except
More informationNew York State Student Learning Objective: Regents Geometry
New York State Student Learning Objective: Regents Geometry All SLOs MUST include the following basic components: Population These are the students assigned to the course section(s) in this SLO all students
More informationXray diffraction techniques for thin films
Xray diffraction techniques for thin films Rigaku Corporation Application Laboratory Takayuki Konya 1 Today s contents (PM) Introduction Xray diffraction method OutofPlane InPlane Pole figure Reciprocal
More informationXRay Diffraction. wavelength Electric field of light
Light is composed of electromagnetic radiation with an electric component that modulates versus time perpendicular to the direction it is travelling (the magnetic component is also perpendicular to the
More informationCentroid: The point of intersection of the three medians of a triangle. Centroid
Vocabulary Words Acute Triangles: A triangle with all acute angles. Examples 80 50 50 Angle: A figure formed by two noncollinear rays that have a common endpoint and are not opposite rays. Angle Bisector:
More informationChapter 7: Basics of Xray Diffraction
Providing Solutions To Your Diffraction Needs. Chapter 7: Basics of Xray Diffraction Scintag has prepared this section for use by customers and authorized personnel. The information contained herein is
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationIntroduction to Powder XRay Diffraction History Basic Principles
Introduction to Powder XRay Diffraction History Basic Principles Folie.1 History: Wilhelm Conrad Röntgen Wilhelm Conrad Röntgen discovered 1895 the Xrays. 1901 he was honoured by the Noble prize for
More informationPennsylvania System of School Assessment
Pennsylvania System of School Assessment The Assessment Anchors, as defined by the Eligible Content, are organized into cohesive blueprints, each structured with a common labeling system that can be read
More informationSolutions to Exercises, Section 5.1
Instructor s Solutions Manual, Section 5.1 Exercise 1 Solutions to Exercises, Section 5.1 1. Find all numbers t such that ( 1 3,t) is a point on the unit circle. For ( 1 3,t)to be a point on the unit circle
More informationPolarization of Light
Polarization of Light References Halliday/Resnick/Walker Fundamentals of Physics, Chapter 33, 7 th ed. Wiley 005 PASCO EX997A and EX999 guide sheets (written by Ann Hanks) weight Exercises and weights
More informationHigher Education Math Placement
Higher Education Math Placement Placement Assessment Problem Types 1. Whole Numbers, Fractions, and Decimals 1.1 Operations with Whole Numbers Addition with carry Subtraction with borrowing Multiplication
More informationPrentice Hall Mathematics Courses 13 Common Core Edition 2013
A Correlation of Prentice Hall Mathematics Courses 13 Common Core Edition 2013 to the Topics & Lessons of Pearson A Correlation of Courses 1, 2 and 3, Common Core Introduction This document demonstrates
More informationBedford, Fowler: Statics. Chapter 4: System of Forces and Moments, Examples via TK Solver
System of Forces and Moments Introduction The moment vector of a force vector,, with respect to a point has a magnitude equal to the product of the force magnitude, F, and the perpendicular distance from
More informationApplications of New, High Intensity XRay Optics  Normal and thin film diffraction using a parabolic, multilayer mirror
Applications of New, High Intensity XRay Optics  Normal and thin film diffraction using a parabolic, multilayer mirror Stephen B. Robie scintag, Inc. 10040 Bubb Road Cupertino, CA 95014 Abstract Corundum
More informationINTERFERENCE OF SOUND WAVES
1/2016 Sound 1/8 INTERFERENCE OF SOUND WAVES PURPOSE: To measure the wavelength, frequency, and propagation speed of ultrasonic sound waves and to observe interference phenomena with ultrasonic sound waves.
More informationFactoring Patterns in the Gaussian Plane
Factoring Patterns in the Gaussian Plane Steve Phelps Introduction This paper describes discoveries made at the Park City Mathematics Institute, 00, as well as some proofs. Before the summer I understood
More informationFraunhofer Diffraction
Physics 334 Spring 1 Purpose Fraunhofer Diffraction The experiment will test the theory of Fraunhofer diffraction at a single slit by comparing a careful measurement of the angular dependence of intensity
More informationProcessing Data with rsmap3d Software Services Group Advanced Photon Source Argonne National Laboratory
Processing Data with rsmap3d Software Services Group Advanced Photon Source Argonne National Laboratory Introduction rsmap3d is an application for producing 3D reciprocal space maps from xray diffraction
More informationPhysics 25 Exam 3 November 3, 2009
1. A long, straight wire carries a current I. If the magnetic field at a distance d from the wire has magnitude B, what would be the the magnitude of the magnetic field at a distance d/3 from the wire,
More informationGeometry Enduring Understandings Students will understand 1. that all circles are similar.
High School  Circles Essential Questions: 1. Why are geometry and geometric figures relevant and important? 2. How can geometric ideas be communicated using a variety of representations? ******(i.e maps,
More informationChapter 2 Laser Diode Beam Propagation Basics
Chapter 2 Laser Diode Beam Propagation Basics Abstract Laser diode beam propagation characteristics, the collimating and focusing behaviors and the M 2 factor are discussed using equations and graphs.
More informationPARALLEL BEAM METHODS IN POWDER DIFFRACTION AND TEXTURE IN THE LABORATORY.
Copyright(c)JCPDSInternational Centre for Diffraction Data 2000,Advances in Xray Analysis,Vol.43 135 PARALLEL BEAM METHODS IN POWDER DIFFRACTION AND TEXTURE IN THE LABORATORY. R.A. Clapp and M.Halleti
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationCommon Core Unit Summary Grades 6 to 8
Common Core Unit Summary Grades 6 to 8 Grade 8: Unit 1: Congruence and Similarity 8G18G5 rotations reflections and translations,( RRT=congruence) understand congruence of 2 d figures after RRT Dilations
More informationFor example, estimate the population of the United States as 3 times 10⁸ and the
CCSS: Mathematics The Number System CCSS: Grade 8 8.NS.A. Know that there are numbers that are not rational, and approximate them by rational numbers. 8.NS.A.1. Understand informally that every number
More informationALGEBRA I / ALGEBRA I SUPPORT
Suggested Sequence: CONCEPT MAP ALGEBRA I / ALGEBRA I SUPPORT August 2011 1. Foundations for Algebra 2. Solving Equations 3. Solving Inequalities 4. An Introduction to Functions 5. Linear Functions 6.
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationPrentice Hall Algebra 2 2011 Correlated to: Colorado P12 Academic Standards for High School Mathematics, Adopted 12/2009
Content Area: Mathematics Grade Level Expectations: High School Standard: Number Sense, Properties, and Operations Understand the structure and properties of our number system. At their most basic level
More informationName Class. Date Section. Test Form A Chapter 11. Chapter 11 Test Bank 155
Chapter Test Bank 55 Test Form A Chapter Name Class Date Section. Find a unit vector in the direction of v if v is the vector from P,, 3 to Q,, 0. (a) 3i 3j 3k (b) i j k 3 i 3 j 3 k 3 i 3 j 3 k. Calculate
More informationDOSIMETRIC CHARACTERIZATION OF DYED PMMA SOLID DOSIMETERS FOR GAMMA RADIATION
2005 International Nuclear Atlantic Conference  INAC 2005 Santos, SP, Brazil, August 28 to September 2, 2005 ASSOCIAÇÃO BRASILEIRA DE ENERGIA NUCLEAR  ABEN ISBN: 8599141015 DOSIMETRIC CHARACTERIZATION
More informationThis is an authordeposited version published in: http://sam.ensam.eu Handle ID:.http://hdl.handle.net/10985/10324
Science Arts & Métiers (SAM) is an open access repository that collects the work of Arts et Métiers ParisTech researchers and makes it freely available over the web where possible. This is an authordeposited
More informationName Geometry Exam Review #1: Constructions and Vocab
Name Geometry Exam Review #1: Constructions and Vocab Copy an angle: 1. Place your compass on A, make any arc. Label the intersections of the arc and the sides of the angle B and C. 2. Compass on A, make
More informationAlgebra 1 2008. Academic Content Standards Grade Eight and Grade Nine Ohio. Grade Eight. Number, Number Sense and Operations Standard
Academic Content Standards Grade Eight and Grade Nine Ohio Algebra 1 2008 Grade Eight STANDARDS Number, Number Sense and Operations Standard Number and Number Systems 1. Use scientific notation to express
More informationCoordinated, Interactive Data Visualization for Neutron Scattering Data
Coordinated, Interactive Data Visualization for Neutron Scattering Data D. J. Mikkelson 2, R. L. Mikkelson 2, T. G. Worlton 1, A. Chatterjee 1, J. P. Hammonds 1, P. F. Peterson 1, A. J. Schultz 1 1 Argonne
More informationDOING PHYSICS WITH MATLAB COMPUTATIONAL OPTICS RAYLEIGHSOMMERFELD DIFFRACTION INTEGRAL OF THE FIRST KIND
DOING PHYSICS WITH MATLAB COMPUTATIONAL OPTICS RAYLEIGHSOMMERFELD DIFFRACTION INTEGRAL OF THE FIRST KIND THE THREEDIMENSIONAL DISTRIBUTION OF THE RADIANT FLUX DENSITY AT THE FOCUS OF A CONVERGENCE BEAM
More information* This work is an official contribution of the National Institute of Standards and Technology and
Variability in the Geometric Accuracy of Additively Manufactured Test Parts A.L. Cooke and J.A. Soons National Institute of Standards and Technology * Gaithersburg, MD, USA Abstract This paper describes
More informationCommon Core State Standards for Mathematics Accelerated 7th Grade
A Correlation of 2013 To the to the Introduction This document demonstrates how Mathematics Accelerated Grade 7, 2013, meets the. Correlation references are to the pages within the Student Edition. Meeting
More informationGeometry Notes PERIMETER AND AREA
Perimeter and Area Page 1 of 57 PERIMETER AND AREA Objectives: After completing this section, you should be able to do the following: Calculate the area of given geometric figures. Calculate the perimeter
More informationMODELING AND IMPLEMENTATION OF THE MECHANICAL SYSTEM AND CONTROL OF A CT WITH LOW ENERGY PROTON BEAM
MODELING AND IMPLEMENTATION OF THE MECHANICAL SYSTEM AND CONTROL OF A CT WITH LOW ENERGY PROTON BEAM João Antônio Palma Setti, j.setti@pucpr.br Pontifícia Universidade Católica do Paraná / Rua Imaculada
More informationTWODIMENSIONAL TRANSFORMATION
CHAPTER 2 TWODIMENSIONAL TRANSFORMATION 2.1 Introduction As stated earlier, Computer Aided Design consists of three components, namely, Design (Geometric Modeling), Analysis (FEA, etc), and Visualization
More informationCopyright 2011 Casa Software Ltd. www.casaxps.com. Centre of Mass
Centre of Mass A central theme in mathematical modelling is that of reducing complex problems to simpler, and hopefully, equivalent problems for which mathematical analysis is possible. The concept of
More informationParallel and Perpendicular. We show a small box in one of the angles to show that the lines are perpendicular.
CONDENSED L E S S O N. Parallel and Perpendicular In this lesson you will learn the meaning of parallel and perpendicular discover how the slopes of parallel and perpendicular lines are related use slopes
More informationNEW YORK STATE TEACHER CERTIFICATION EXAMINATIONS
NEW YORK STATE TEACHER CERTIFICATION EXAMINATIONS TEST DESIGN AND FRAMEWORK September 2014 Authorized for Distribution by the New York State Education Department This test design and framework document
More informationGRAPHING (2 weeks) Main Underlying Questions: 1. How do you graph points?
GRAPHING (2 weeks) The Rectangular Coordinate System 1. Plot ordered pairs of numbers on the rectangular coordinate system 2. Graph paired data to create a scatter diagram 1. How do you graph points? 2.
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More informationSome Comments on the Derivative of a Vector with applications to angular momentum and curvature. E. L. Lady (October 18, 2000)
Some Comments on the Derivative of a Vector with applications to angular momentum and curvature E. L. Lady (October 18, 2000) Finding the formula in polar coordinates for the angular momentum of a moving
More informationTHEORETICAL MECHANICS
PROF. DR. ING. VASILE SZOLGA THEORETICAL MECHANICS LECTURE NOTES AND SAMPLE PROBLEMS PART ONE STATICS OF THE PARTICLE, OF THE RIGID BODY AND OF THE SYSTEMS OF BODIES KINEMATICS OF THE PARTICLE 2010 0 Contents
More informationCalculation of Sourcedetector Solid Angle, Using Monte Carlo Method, for Radioactive Sources with Various Geometries and Cylindrical Detector
International Journal of Pure and Applied Physics ISSN 09731776 Volume 3, Number 2 (2007), pp. 201 208 Research India Publications http://www.ripublication.com/ijpap.htm Calculation of Sourcedetector
More informationExperimental Question 1: Levitation of Conductors in an Oscillating Magnetic Field SOLUTION ( )
a. Using Faraday s law: Experimental Question 1: Levitation of Conductors in an Oscillating Magnetic Field SOLUTION The overall sign will not be graded. For the current, we use the extensive hints in the
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationCRLS Mathematics Department Algebra I Curriculum Map/Pacing Guide
Curriculum Map/Pacing Guide page 1 of 14 Quarter I start (CP & HN) 170 96 Unit 1: Number Sense and Operations 24 11 Totals Always Include 2 blocks for Review & Test Operating with Real Numbers: How are
More informationGeometry of Vectors. 1 Cartesian Coordinates. Carlo Tomasi
Geometry of Vectors Carlo Tomasi This note explores the geometric meaning of norm, inner product, orthogonality, and projection for vectors. For vectors in threedimensional space, we also examine the
More information1.3. DOT PRODUCT 19. 6. If θ is the angle (between 0 and π) between two nonzero vectors u and v,
1.3. DOT PRODUCT 19 1.3 Dot Product 1.3.1 Definitions and Properties The dot product is the first way to multiply two vectors. The definition we will give below may appear arbitrary. But it is not. It
More informationThnkwell s Homeschool Precalculus Course Lesson Plan: 36 weeks
Thnkwell s Homeschool Precalculus Course Lesson Plan: 36 weeks Welcome to Thinkwell s Homeschool Precalculus! We re thrilled that you ve decided to make us part of your homeschool curriculum. This lesson
More informationCurriculum Map by Block Geometry Mapping for Math Block Testing 20072008. August 20 to August 24 Review concepts from previous grades.
Curriculum Map by Geometry Mapping for Math Testing 20072008 Pre s 1 August 20 to August 24 Review concepts from previous grades. August 27 to September 28 (Assessment to be completed by September 28)
More informationGrazing incidence wavefront sensing and verification of Xray optics performance
Grazing incidence wavefront sensing and verification of Xray optics performance Timo T. Saha, Scott Rohrbach, and William W. Zhang, NASA Goddard Space Flight Center, Greenbelt, Md 20771 Evaluation of
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationGuide to Understanding Xray Crystallography
Guide to Understanding Xray Crystallography What is Xray Crystallography and why do I need to learn it? Xray Crystallography is a scientific method of determining the precise positions/arrangements
More informationGeometry. Higher Mathematics Courses 69. Geometry
The fundamental purpose of the course is to formalize and extend students geometric experiences from the middle grades. This course includes standards from the conceptual categories of and Statistics and
More informationQuick Guide for Data Collection on the NIU Bruker Smart CCD
Quick Guide for Data Collection on the NIU Bruker Smart CCD 1. Create a new project 2. Optically align the crystal 3. Take rotation picture 4. Collect matrix to determine unit cell 5. Refine unit cell
More informationWORK SCHEDULE: MATHEMATICS 2007
, K WORK SCHEDULE: MATHEMATICS 00 GRADE MODULE TERM... LO NUMBERS, OPERATIONS AND RELATIONSHIPS able to recognise, represent numbers and their relationships, and to count, estimate, calculate and check
More informationDiffraction Course Series 2015
Diffraction Course Series 2015 Mark Wainwright Analytical Centre Kensington Campus, Chemical Sciences Building F10, Room G37 The Mark Wainwright Analytical Centre is offering a new series of courses covering
More informationA Game of Numbers (Understanding Directivity Specifications)
A Game of Numbers (Understanding Directivity Specifications) José (Joe) Brusi, Brusi Acoustical Consulting Loudspeaker directivity is expressed in many different ways on specification sheets and marketing
More informationCalculus C/Multivariate Calculus Advanced Placement G/T Essential Curriculum
Calculus C/Multivariate Calculus Advanced Placement G/T Essential Curriculum UNIT I: The Hyperbolic Functions basic calculus concepts, including techniques for curve sketching, exponential and logarithmic
More informationO6: The Diffraction Grating Spectrometer
2B30: PRACTICAL ASTROPHYSICS FORMAL REPORT: O6: The Diffraction Grating Spectrometer Adam Hill Lab partner: G. Evans Tutor: Dr. Peter Storey 1 Abstract The calibration of a diffraction grating spectrometer
More informationInterferometers. OBJECTIVES To examine the operation of several kinds of interferometers. d sin = n (1)
Interferometers The true worth of an experimenter consists in his pursuing not only what he seeks in his experiment, but also what he did not seek. Claude Bernard (18131878) OBJECTIVES To examine the
More informationSolutions to old Exam 1 problems
Solutions to old Exam 1 problems Hi students! I am putting this old version of my review for the first midterm review, place and time to be announced. Check for updates on the web site as to which sections
More information